# SAE-AISI 1335 (G13350) Carbon Steel

SAE-AISI 1335 steel is a resulfurized carbon steel formulated for primary forming into wrought products. Cited properties are appropriate for the annealed condition. 1335 is the designation in both the SAE and AISI systems for this material. G13350 is the UNS number.

The graph bars on the material properties cards below compare SAE-AISI 1335 steel to: wrought resulfurized carbon steels (top), all iron alloys (middle), and the entire database (bottom). A full bar means this is the highest value in the relevant set. A half-full bar means it's 50% of the highest, and so on.

## Mechanical Properties

Brinell Hardness

160

Elastic (Young's, Tensile) Modulus

190 *GPa* 27 *x 10 ^{6} psi*

Elongation at Break

23 *%*

Fatigue Strength

220 *MPa* 32 *x 10 ^{3} psi*

Poisson's Ratio

0.29

Shear Modulus

73 *GPa* 11 *x 10 ^{6} psi*

Shear Strength

350 *MPa* 50 *x 10 ^{3} psi*

Tensile Strength: Ultimate (UTS)

550 *MPa* 79 *x 10 ^{3} psi*

Tensile Strength: Yield (Proof)

300 *MPa* 44 *x 10 ^{3} psi*

## Thermal Properties

Latent Heat of Fusion

250 *J/g*

Maximum Temperature: Mechanical

400 *°C* 750 *°F*

Melting Completion (Liquidus)

1460 *°C* 2650 *°F*

Melting Onset (Solidus)

1410 *°C* 2580 *°F*

Specific Heat Capacity

470 *J/kg-K* 0.11 *BTU/lb-°F*

Thermal Conductivity

51 *W/m-K* 30 *BTU/h-ft-°F*

Thermal Expansion

12 *µm/m-K*

## Electrical Properties

Electrical Conductivity: Equal Volume

7.2 *% IACS*

Electrical Conductivity: Equal Weight (Specific)

8.3 *% IACS*

## Otherwise Unclassified Properties

Base Metal Price

1.9 *% relative*

Density

7.8 *g/cm ^{3}* 490

*lb/ft*

^{3}Embodied Carbon

1.4 *kg CO _{2}/kg material*

Embodied Energy

19 *MJ/kg* 8.1 *x 10 ^{3} BTU/lb*

Embodied Water

48 *L/kg* 5.7 *gal/lb*

## Common Calculations

Resilience: Ultimate (Unit Rupture Work)

110 *MJ/m ^{3}*

Resilience: Unit (Modulus of Resilience)

250 *kJ/m ^{3}*

Stiffness to Weight: Axial

13 *points*

Stiffness to Weight: Bending

24 *points*

Strength to Weight: Axial

19 *points*

Strength to Weight: Bending

19 *points*

Thermal Diffusivity

14 *mm ^{2}/s*

Thermal Shock Resistance

17 *points*

## Alloy Composition

Fe | 97.3 to 97.9 | |

Mn | 1.6 to 1.9 | |

C | 0.33 to 0.38 | |

Si | 0.15 to 0.35 | |

S | 0 to 0.040 | |

P | 0 to 0.035 |

All values are % weight. Ranges represent what is permitted under applicable standards.

## Followup Questions

## Similar Alloys

## Further Reading

ASTM A752: Standard Specification for General Requirements for Wire Rods and Coarse Round Wire, Alloy Steel

ASTM A322: Standard Specification for Steel Bars, Alloy, Standard Grades

Carbon Steel Handbook, D. Gandy, 2007

ASM Specialty Handbook: Carbon and Alloy Steels, J. R. Davis (editor), 1996

Ferrous Materials: Steel and Cast Iron, Hans Berns and Werner Theisen, 2008

Steels: Processing, Structure, and Performance, 2nd ed., George Krauss, 2015